| ||Format||Pages||Price|| |
|8||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$52.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$62.00||  ADD TO CART|
Significance and Use
5.1 Decomposition of a plastic within a landfill involves processes in aerobic and anaerobic environmental conditions that can affect the decomposition of other materials enclosed by or in close proximity to the plastic. The rate of change from aerobic to anaerobic conditions is probably a characteristic of the particular landfill site, its garbage and the filling technique and is therefore difficult to assess with any degree of accuracy. Different sources indicate days to months (Refs ( and )() for this change with the spread dependent on the perspective of what is aerobic or anaerobic and how fast the environment changes, 30 days is chosen in this method as a compromise time period. (Note, even very low levels of oxygen, far below normal atmospheric concentration can promote oxidative degradation). Obviously, there will be pockets of protected (in bags, cans, etc.) aerobic activity enclosed in any landfill. There is currently no evidence or data to support claims that rapid degradation of the plastic (when compared to conventional non-degradable plastic) can increase the economic feasibility of landfill-gas recovery, minimize the duration of after-care of the landfill, and make possible the recovery of the volume reduction of the waste due to degradation and biodegradation during the active life of the landfill. Additionally, it is possible that the rapid degradation and biodegradation of plastics can create hazardous conditions in landfills, such as the shifting of cells and overall stability. This standard method has been developed to permit determination of the aerobic degradation and anaerobic biodegradation of plastic products when placed in biologically active environments simulating some landfill conditions. )
5.2 The decomposition of plastic materials in a landfill is of importance, as most landfills are biologically active and are an increasingly significant source of renewable energy. As degradation occurs in a landfill, it is of immediate concern that the plastic materials do not produce toxic metabolites or end products under the various conditions that occur in a landfill. The mixtures remaining after completion of the test method, containing fully or partially degraded plastic materials or extracts can be, when appropriate, submitted subsequently to ecotoxicity testing, see Practice and Guide for details, in order to assess the environmental hazards posed by the breakdown of plastics to varying degrees in landfills, especially if leaching occurs. This test method has been designed to assess aerobic degradation and anaerobic biodegradation under optimum and less-than-optimum conditions and toxicity.
5.3 Limitations—Because a wide variation exists in the construction and operation of landfills, and because regulatory requirements for landfills vary greatly, this procedure is not intended to simulate the environments of all landfills. However, it is expected to closely resemble the environment of a biologically active landfill. More specifically, the procedure is intended to create a standard laboratory environment that permits rapid and reproducible determination of the aerobic degradability and anaerobic biodegradability under accelerated landfill conditions, while at the same time producing reproducible mixtures of fully and partially decomposed household waste with plastic materials for ecotoxicological assessment.
1.1 This test method is used to determine the degree and rate of aerobic degradation (as indicated by loss of tensile strength, molecular weight, possibly resulting in disintegration and fragmentation) and anaerobic biodegradation of plastic materials in an accelerated aerobic-anaerobic bioreactor landfill test environment. It can simulate the change from aerobic to anaerobic environments over time as landfill depth increases. In Tier 1, the test plastic material is mixed with household waste, then pretreated and stabilized aerobically in the presence of air, in a sealed vessel in a temperature range that is consistent with the average temperature range of those recorded for landfills. The tier is an accelerated simulation of degradation with concomitant oxygen consumption and depletion with time as if oxidative degradation proceeds. In Tier 2 samples of the plastic materials pretreated aerobically as described in Tier 1, are exposed to a methanogenic inoculum derived from anaerobic digesters operating only on pretreated household waste. The anaerobic decomposition and biodegradation occur under dry (more than 30 % total solids) and static non-mixed conditions.
1.2 This test method generates comparative data for several materials and must not be used to make claims regarding benefits of placing degradable or biodegradable plastics in landfills. Claims must be limited to and dependent on the results obtained from each tier.
1.2.1 If only Tier 1 is run, then the claims must state: Will modify the performance/physical properties (for example, mechanical properties will degrade), up to a measured percent, X%, in a given time period, Y days using Test Methods (Molecular weight change) and Test Method (tensile strength change) in a biologically active “bioreactor” landfill. Report measured percent property changes and standards used to measure the test results which are, for example, changes in tensile strength, mass and molecular weight, as well as residual particle size ranges in Section to support the extent of such claims.
1.2.2 If both Tier 1 and Tier 2 are run, then claims shall state: Will biodegrade in a biologically active “bioreactor” landfill to a degree, X%, in Y days established by the test results based on the extent to which the plastic sample is converted to gaseous carbon in the form of carbon dioxide and methane and this shall be made available according to Section to support the extent of such claims. It should be noted that biodegradation testing is very dependent on conditions chosen in this laboratory test and may well vary widely when the test is run with different inoculum, The results reported pertain only to the test conditions run and do not rule out potential biodegradation under other conditions and real world environments.
1.3 Tier 1 of this test method is designed to estimate the aerobic degradation of plastics, that is disintegration and fragmentation, only, by measuring the loss of physical and chemical properties of said plastics. The test environment is then changed to that of Tier 2, an anaerobic condition, and biodegradation is measured by a combination of evolved carbon dioxide and methane gases as a percentage of the conversion of carbon in the plastic sample to carbon in the gaseous form under conditions that resemble landfill conditions. This test method does not simulate all conditions found in landfills, especially those found in biologically inactive landfills. This test method more closely resembles those types of bioreactor landfills in which the gas generated is recovered or even actively promoted, or both, for example, by inoculation (co-deposition of anaerobic sewage sludge and anaerobic leachate recirculation), moisture control in the landfill (leachate recirculation), and temperature control (short-term injection of oxygen and heating of re-circulated leachate) (. )
1.4 This test method produces partially degraded mixtures of municipal solid waste and plastics that, where required, are used to assess the ecotoxicological risks associated with the degradation of plastics after various stages of aerobic degradation and anaerobic biodegradation in a landfill.
1.5 The intended use of this method is for a comparison and ranking of aerobic degradation and anaerobic biodegradation of plastics after disposal in a bioreactor landfill. It is not designed or intended to be used to support claims recommending the value of plastic degradation in full-scale landfills. This simulation of an active landfill allows measurement of the percentage of aerobic degradation and anaerobic biodegradation (biogas evolution) in specified time periods, only.
1.6 Though the test method is in two tiers, they are meant to simulate a real world cycle of degradation in a landfill and are most preferably run consecutively and not independently or separately.
1.7 It is cautioned that the results of any laboratory landfill simulation cannot be directly extrapolated to actual disposal environments: confirmation to real world exposure is ultimately required as with all ASTM Standards. This confirmation is essential for landfill as the types of landfills vary widely, some are even heavily lined, tombs, and these will limit degradation severely.
1.8 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.9 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
Note 1: There is no known ISO equivalent to this standard.
1.10 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D618 Practice for Conditioning Plastics for Testing
D883 Terminology Relating to Plastics
D1293 Test Methods for pH of Water
D1888 Methods Of Test for Particulate and Dissolved Matter in Water
D2908 Practice for Measuring Volatile Organic Matter in Water by Aqueous-Injection Gas Chromatography
D3590 Test Methods for Total Kjeldahl Nitrogen in Water
D3593 Test Method for Molecular Weight Averages/ Distribution of Certain Polymers by Liquid Size-Exclusion Chromatography (Gel Permeation Chromatography GPC) Using Universal Calibration
D3826 Practice for Determining Degradation End Point in Degradable Polyethylene and Polypropylene Using a Tensile Test
D4129 Test Method for Total and Organic Carbon in Water by High Temperature Oxidation and by Coulometric Detection
D5526 Test Method for Determining Anaerobic Biodegradation of Plastic Materials Under Accelerated Landfill Conditions
D5951 Practice for Preparing Residual Solids Obtained After Biodegradability Standard Methods for Plastics in Solid Waste for Toxicity and Compost Quality Testing
D6954 Guide for Exposing and Testing Plastics that Degrade in the Environment by a Combination of Oxidation and Biodegradation
E260 Practice for Packed Column Gas Chromatography
E355 Practice for Gas Chromatography Terms and Relationships
APHA-AWWA-WPCF Standards2540D Total Suspended Solids Dried at 103105C 2540E Fixed and Volatile Solids Ignited at 550C
ICS Number Code 13.030.40 (Installations and equipment for waste disposal and treatment)
UNSPSC Code 13100000(Rubber and elastomers)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D7475-20, Standard Test Method for Determining the Aerobic Degradation and Anaerobic Biodegradation of Plastic Materials under Accelerated Bioreactor Landfill Conditions, ASTM International, West Conshohocken, PA, 2020, www.astm.orgBack to Top